**1. Introduction**

Polymer Optical fiber (POF) is one kind of optical fiber made of polymer material. It has attractive characteristics such as low Young's modulus, high strain, high flexibility, and biocompatibility performance compared with silica optical fiber. The first commercially polymer optical fiber with deuterated polymer was reported in the early 1960s [1]. From the 1950s, optical fibers are under research due to the demand of transmission high-speed data. Silica fibers were also under intense research since their first proposal as a transmission medium by Kao et al. [2]. At that time the transmission loss of silica fibers was high and the theoretical predictions allow to propose pure glass as fiber material able to transmit light over a hundred kilometers. Then, the purity of silica material was significantly improved and losses were reduced up to 0.5 dB/km at 1300 nm, and 0.2 dB/km at 1550 nm after a few years [3]. Therefore, most of the research was shift to the silica optical fiber based transmission system, which forms the backbone of the modern telecommunications systems [4], the transmission loss of silica optical fiber, PMMA POF and CYTOP POF from 400 nm to 1600 nm wavelength shown in **Figure 1**.

The absorption loss of silica material is lower compared with polymer material although Rayleigh scattering is the main mechanism for both cases. The main absorption of polymer material contribution is due to the harmonics of the C-H vibration [5]. Researchers and companies in Japan did intense work to reduce the transmission loss of PMMA POF, also investigated perfluorinated polymer fibers (GI-POF) with

#### **Figure 1.**

*The transmission loss of silica optical fiber, PMMA POF and CYTOP POF, and from 400 nm to 1600 nm wavelength.*

lower losses, which shown 50 dB/km loss over 650 nm ~ 1300 nm wavelength [6–8]. However, the fabrication expend of the fluorinated polymer optical fiber are still higher compared with silica optical fiber. So, the most common material for polymer optical fiber is still PMMA which is cheap with high transmission loss at the telecom band. Both GI-POF and step-index POF mentioned above are multimode fibers, until now the main commercial POFs with single-mode performance with low fabrication cost still under research.

In recent years, the use of POFs for varies sensing applications under research are growing [9–13]. Sensing technology based on POF are mainly divided into intensity modulation technology, Brillouin scattering technology, Grating devices technology. Intensity modulation technology is the basic optical fiber sensing technologies, the main disadvantage is the performance related to the stability of the photo detector and the source, which always introduces errors in the measurement [14]. Brillouin scattering is an attractive sensing technology based on optical fiber which has been explored with silica optical fiber for many years [15]. POF with the advantage such as high flexibility can be exploited under large strains. Brillouin scattering technology in POF are good candidate for structural health monitoring. Grating devices technology as one of the main sensing technologies in silica fiber with high resolution and repeatable performance already goes from lab to the industry [16–18]. Although the first FBG in POF was reported by Peng's group with a stepindex polymer optical fiber before twenty years [19], one main challenge for grating device fabrication in POF is the multimode performance of fiber, make it is difficult to analyses the spectrum from different modes.

The mature of photonic crystal fiber (PCF) technology and the excellent performance of PCF attracted the attention of the researcher for POF fabrication and application, which was invested with silica structures in 1997 [20]. The Large et al. obtained the first PCF with polymer material with endless single-mode performance in 2001 [21]. Then, H. Dobb et al. [22] reported the first FBG in endless single-mode mPOF in 2005, open the research of grating devices fabrication research with POF. Different materials such as Zeonex [23, 24], TOPAS [25, 26], and polycarbonate [27, 28] were used to fabricate microstructured polymer optical fiber (mPOF), different kind of laser irradiation technology were investigated for POG

**31**

**Figure 2.**

*Fabrication and Application of Polymer Optical Fiber Grating Devices*

grating devices fabrication. Special grating such as Uniform FBG, Phase-shift FBG,

In this chapter, we report the basic theory of grating devices, and the lasted results about POF grating devices fabrication and potential applications. Section 2 will focus on the basic theory of grating devices such as FBG and LPG. Recent results on POF gratings fabrication with different kind of fibers and UV lasers will be reported in Section 3 and Section 4 will focus on introduce the potential applications of POF grating devices. Finally, the last section summarizes the main

Grating devices in optical fibers normally belong to two main types, which depending on the mode-coupling mechanism, counter-directional coupling is the responsible mechanism in fiber Bragg gratings (FBGs) and co-directional coupling

FBG is a device due to periodic modulation of the refractive index along the optical fiber, normally obtained through the exposure of the optical fiber core with an intense optical interference pattern [29]. The periodic structure in an FBGs as a selective mirror, and the wavelength satisfies the Bragg condition expressed as:

where neff is the average effective refractive index along the fiber and Ʌ is the grating period. Then, **Figure 2** shown a component reflects one wavelength and transmits all others with a wavelength-specific dielectric mirror response.

The ability of the FBGs shown optical communication applications such as band stop filters in Raman amplifiers [30] dispersion compensators [31], and wavelength division multiplexers [32]. Also, FBG can be used for sensing purposes, such as

As **Figure 3** shown, LPG is based on a periodic modulation of the refractive index of the fiber core along of the direction of propagation of the light, and the core mode couples to co-propagating cladding modes, different attenuation bands

are obtained when the resonance condition is satisfied the equation below:

*The transmission and reflection spectrum of a broad light go through one fiber with FBG inside.*

λ= Λ Bragg eff 2*n* (1)

λ =Λ∗∆ res n (2)

Tilted FBG, Chirped FBG, LPG is investigated for various applications.

*DOI: http://dx.doi.org/10.5772/intechopen.94351*

**2. The basic theory of POF grating devices**

as main mechanism for long-period gratings (LPG).

humidity, strain and temperature measurements.

conclusions.

#### *Fabrication and Application of Polymer Optical Fiber Grating Devices DOI: http://dx.doi.org/10.5772/intechopen.94351*

*Application of Optical Fiber in Engineering*

cost still under research.

**Figure 1.**

*wavelength.*

to analyses the spectrum from different modes.

lower losses, which shown 50 dB/km loss over 650 nm ~ 1300 nm wavelength [6–8]. However, the fabrication expend of the fluorinated polymer optical fiber are still higher compared with silica optical fiber. So, the most common material for polymer optical fiber is still PMMA which is cheap with high transmission loss at the telecom band. Both GI-POF and step-index POF mentioned above are multimode fibers, until now the main commercial POFs with single-mode performance with low fabrication

*The transmission loss of silica optical fiber, PMMA POF and CYTOP POF, and from 400 nm to 1600 nm* 

In recent years, the use of POFs for varies sensing applications under research are growing [9–13]. Sensing technology based on POF are mainly divided into intensity modulation technology, Brillouin scattering technology, Grating devices technology. Intensity modulation technology is the basic optical fiber sensing technologies, the main disadvantage is the performance related to the stability of the photo detector and the source, which always introduces errors in the measurement [14]. Brillouin scattering is an attractive sensing technology based on optical fiber which has been explored with silica optical fiber for many years [15]. POF with the advantage such as high flexibility can be exploited under large strains. Brillouin scattering technology in POF are good candidate for structural health monitoring. Grating devices technology as one of the main sensing technologies in silica fiber with high resolution and repeatable performance already goes from lab to the industry [16–18]. Although the first FBG in POF was reported by Peng's group with a stepindex polymer optical fiber before twenty years [19], one main challenge for grating device fabrication in POF is the multimode performance of fiber, make it is difficult

The mature of photonic crystal fiber (PCF) technology and the excellent performance of PCF attracted the attention of the researcher for POF fabrication and application, which was invested with silica structures in 1997 [20]. The Large et al. obtained the first PCF with polymer material with endless single-mode performance in 2001 [21]. Then, H. Dobb et al. [22] reported the first FBG in endless single-mode mPOF in 2005, open the research of grating devices fabrication research with POF. Different materials such as Zeonex [23, 24], TOPAS [25, 26], and polycarbonate [27, 28] were used to fabricate microstructured polymer optical fiber (mPOF), different kind of laser irradiation technology were investigated for POG

**30**

grating devices fabrication. Special grating such as Uniform FBG, Phase-shift FBG, Tilted FBG, Chirped FBG, LPG is investigated for various applications.

In this chapter, we report the basic theory of grating devices, and the lasted results about POF grating devices fabrication and potential applications. Section 2 will focus on the basic theory of grating devices such as FBG and LPG. Recent results on POF gratings fabrication with different kind of fibers and UV lasers will be reported in Section 3 and Section 4 will focus on introduce the potential applications of POF grating devices. Finally, the last section summarizes the main conclusions.
